Silver-antimony-telluride (AgSbTe2) based compounds have emerged as a promising class of materials for thermoelectric (TE) power generation at the mid-temperature range. This Chapter demonstrates utilization of first-principles calculations for predicting TE properties of AgSbTe2-based compounds and experimental validations. Predictive calculations of the effects of La-doping on vibrational and electronic properties of AgSbTe2 compounds are performed applying the density functional theory (DFT), and temperature-dependent TE transport coefficients are evaluated applying the Boltzmann transport theory (BTE). Experimentally, model ternary (AgSbTe2) and quaternary (3 at. % La-AgSbTe2) compounds were synthesized, for which TE transport coefficients were measured, indicating that thermal conductivity decreases due to La-alloying. The latter also reduces electrical conductivity and increases Seebeck coefficients. All trends correspond with those predicted from first-principles. Thermal stability issues are essential for TE device operation at service conditions, e.g. changes of matrix composition and second-phase precipitation, and are also addressed in this study on both computational and experimental aspects. It is shown that La-alloying affects TE figure-of-merit positively, e.g., improving from 0.35 up to 0.50 at 260 °C. We highlight the universal aspects of this approach that can be applied for other TE compounds. This enables us screening their performance prior to synthesis in laboratory.
- first-principles calculations
- thermoelectric transport properties
- Boltzmann transport theory
- lattice dynamics
- thermal stability
It is of utmost technological importance to develop predictive tools that will provide us with information about design of materials' functional properties. In this context, density functional theory (DFT) first-principle calculations offer us such possibilities [1–4], allowing us calculation of structural, interfacial, vibrational, and electronic properties. Knowledge of these properties and how they depend on temperature and material’s composition are essential to assess total thermoelectric (TE) performance of thermoelectric device. Among recently investigated TE materials, silver-antimony-telluride (AgSbTe2)-based alloys have emerged as a promising class of materials for TE power generation in low- to mid-temperature range. These compounds are derivatives of lead-antimony-silver-telluride (LAST)-based alloys of AgPbmSbTe2+m form [5–9], which exhibit large TE figure-of-merit
AgSbTe2-based alloys serve not only for TE power conversion or cooling, but also for nonvolatile electronic memory, being classified as phase change materials, as demonstrated in thorough investigation by Wuttig and coworkers [12–15]. They have attracted scientific interest owing to their special nature of interatomic bonding and vibrational properties [16–18]. On TE aspect, their superior performance is associated mainly to glass-like, intrinsically low values of lattice thermal conductivities, as low as 0.6 W m−1 K−1 . This anomaly is associated either to strong anharmonicity of interatomic forces [20, 21] or to relatively large variance of interatomic forces prevailing between Ag+ and Sb3+ cations, encouraging phonon scattering . Additionally, resonant bonding yields high level of structural instability, that is accompanied, for instance, by spontaneous phase decomposition [23, 24]. This, intriguingly, what makes AgSbTe2-based alloys good materials for both TE and phase change applications. Owing to these peculiarities, these alloys have recently been investigated extensively, either experimentally [19, 25–30] or computationally [18, 22, 31–33].
Despite of relatively high
Among efforts to improve TE properties of AgSbTe2-based alloys, Min et al. reported on improvement of electron transport properties due to La-doping . Positive effects on PbTe compound due to La-doping were recorded, as well [54, 55]. In their recent study, Min et al. introduce a complete analysis of TE properties of AgSbTe2 doped with La of different concentrations .
Notwithstanding the aforementioned successful experimental and computational attempts, a set of experimental routines, that is initiated and directed by predictions from first principles for complete TE performance or any other computational procedure, is missing.
A significant step in this direction is introduced by our previous investigations of AgSbTe2-based phase, involving both computational and experimental aspects [57, 58]. Vibrational properties of both AgSbTe2-based and La-doped-AgSbTe2 alloys, including frequency-dependent vibrational density of states functions (v-DOS), temperature-dependent heat capacity, sound velocities, and Debye temperatures were evaluated employing lattice dynamics first-principles calculations. It was reported that La-doping reduces average sound velocity and varies v-DOS of AgSbTe2-based phase [57, 58]. Quantitatively, lattice thermal conductivity of La0.125Ag0.875SbTe2 alloy was calculated to be lower by ca. 14%, than that of AgSbTe2-based phase at 300 K . Experimental validations of these effects of La-alloying on reducing lattice thermal conductivity were made, as well .
This chapter introduces a refined approach of evaluating temperature-dependent lattice thermal conductivity from data obtained
2. Chapter outline
This chapter consists primarily of original computational and experimental data along with data, that were reported by us earlier [57, 58], and is aimed at drawing a complete picture depicting the role of lanthanum-alloying in silver-antimony-telluride-based alloys on a broad TE view. Herein, we demonstrate how alloying of AgSbTe2 (P4/mmm) alloy with lanthanum solute atoms brings about significant reduction in thermal conductivity with positive effects on TE power factor, as well; thus, achieving improved
Computational procedures are divided into the following steps:
Total energy calculations for different polymorphs of AgSbTe2 phase are implemented to evaluate their Helmholtz free energies, indicating which one is the most stable around and above room temperature.
Vibrational calculations are performed for both La-free and La-doped lattices, including phonon dispersion and density of states, average sound velocity, and Debye temperature. These values enable us evaluating temperature-dependent lattice thermal conductivity values.
Electronic calculations of band structures of both La-free and La-doped lattices are performed, and the resulting transport coefficients are derived applying Boltzmann transport theory.
To consider the case in which Sb2Te3- and Sb8Te3-phases precipitate inside AgSbTe2-matrix, similar DFT transport coefficient calculations are performed for both phases, as well. In this context, the molar formation energies of both phases and the free energies of their interfaces with AgSbTe2-matrix are simulated to predict their thermal stability and nucleation sequence.
Additionally, to address the influence of deviations from AgSbTe2-stoichiometry on electron transport properties, the latter is simulated for two off-stoichiometric model alloys Ag3SbTe4 and AgSb3Te4.
Experimental procedures are divided into the following steps:
Model ternary (AgSbTe2) and quaternary (3 at.% La-AgSbTe2) alloys are synthesized by vacuum melting followed by quenching and hot-pressing. The appropriate conditions enabling formation of AgSbTe2-matrix that dissolves La-atoms with no La-rich precipitates are found.
Differential scanning calorimetry (DSC) tests are implemented for both La-free and La-doped alloys to address thermal stability issues and how they are influenced by La-additions.
Temperature-dependent thermal conductivity of both alloys is determined to realize effects of La-doping and to compare them with those predicted from first-principles.
Similarly, both temperature-dependent electrical conductivity and Seebeck coefficients are measured for ternary and quaternary alloys to realize effects of La-doping and to compare them with those predicted from first-principles.
Finally, to assess whether La-doping contributes to conversion efficiency, TE power factor and figure-of-merit are evaluated for La-free and La-doped materials.
3. Research methods
This section provides a brief description of computational and experimental methods applied in this research.
3.1. First-principles calculation
The primary calculations are performed for AgSbTe2 stoichiometric phase. To address, however, both optional cases of second-phase nucleation and deviations from stoichiometric composition, as described in Section 2, the following phases are simulated, as well: Sb2Te3, Sb8Te3, Ag3SbTe4, and AgSb3Te4.
3.1.1. The base AgSbTe2 phase—structural and vibrational calculations
Silver-antimony-telluride of AgSbTe2 stoichiometry is commonly known to introduce a cubic lattice structure; however, it was suggested, that it may coexist with tetragonal and rhombohedral forms . The following optional space group symmetries: cubic (Pm-3m, No. 221), tetragonal (P4/mmm, No. 123), and rhombohedral (R-3m, No. 166) have been simulated from first-principles . Calculations of temperature-dependent Helmholtz free energy for these three polymorphs indicate that P4/mmm polymorph is the most stable one at temperatures above 400 K, whose energy exhibits close proximity to that of Pm-3m polymorph. Based on calculated v-DOS function for P4/mmm model alloy consisting of 4 atoms per simulation cell, Figure 1a, it was decided to test effects of doping with lanthanum atoms (to be discussed further below). To represent effects of La-doping with effective concentration of La atoms, that is close to realistic doping levels, a model compound of Ag7LaSb8Te16 stoichiometry was constructed having the same P4/mmm space group symmetry as of the original AgSbTe2 lattice. In this compound, consisting of 32 atoms per simulation cell, Figure 1b, La-atom substitutes for of Ag-atoms, so that, the resulting concentration is 3.125 at.% La. Computational parameters concerning structural relaxation and vibrational properties are provided in detail . The effects of La-doping on vibrational and thermal properties will be discussed further below.
3.1.2. The base AgSbTe2 phase—electronic calculations
To simulate the effects of La-doping on electrical conductivity and Seebeck coefficient, electronic band structures are calculated for both lattices from first principles. A plane-wave basis set is implemented in Vienna
The calculated 0 K band structures are used for evaluation of temperature-dependent electrical conductivity, electronic component of thermal conductivity, and Seebeck coefficient, applying near-equilibrium Boltzmann transport theory with constant relaxation time approximation, as implemented in BoltzTrap code .
The partial electrical conductivity tensor, , represented for
where is characteristic unit cell volume and is equilibrium Fermi-Dirac distribution function . The electronic component of thermal conductivity tensor, , is, accordingly, expressed by:
3.1.3. The Sb2Te3 and Sb8Te3 phases
Nonmagnetic DFT calculations are performed for Sb2Te3 and Sb8Te3 crystal structures having (R-3m) space group symmetry, which incorporate 15 and 33 atoms per simulation cell, respectively. Both lattice structures are rendered in Figure 1
Structural relaxation procedures are first performed, allowing variation of cell volume and atom positions at all degrees of freedom, setting a convergence threshold of 10−4 eV Å−1 for Hellman-Feynman forces. The resulting lattice parameters obtained for relaxed crystal structures are: a = b = 4.34 Å and c = 31.21 Å for Sb2Te3; and: a = b = 4.37 Å and c = 64.93 Å for Sb8Te3, which are in good agreement with data reported in the literature [72, 73]. Then, electronic band structure calculations are performed for both relaxed structures.
Band structures are calculated in the same manner as mentioned above, allowing calculations of temperature-dependent electrical conductivity, electronic component of thermal conductivity, and Seebeck coefficient values. These calculations yield p-type behavior for both structures, and we fine-tune the positions of electronic chemical potential to reside at the top of the valence bands. This yields Seebeck coefficient values that are very similar to those measured by us experimentally for pure Sb2Te3 standard. Additionally, we set electron relaxation time to be 8 fs, so as to fit electrical conductivity values calculated for Sb2Te3 with those measured for the same standards. We, then, apply the same relaxation time for Sb8Te3, as well.
To address bulk and interfacial energetic aspects related with nucleation of Sb2Te3 and Sb8Te3 phases in AgSbTe2 phase, we have simulated formation energies of Sb2Te3 and Sb8Te3 phases and their interfaces with AgSbTe2 phase. Molar formation energy of model SbpTeq cell, , is calculated using the following expression :
where is cell’s molar total energy and and are chemical potentials of Sb- and Te-atoms in their standard states, which are evaluated to be −397.72 and −303.12 kJ mol−1, respectively. The free energy of silver-antimony-telluride (AST)/antimony-telluride (SBT) interface is calculated constructing a slab model having AST/SBT generic form, and using the following expression :
3.1.4. Ag3SbTe4 and AgSb3Te4 model compounds
To simulate the effects of deviations from stoichiometric AgSbTe2 composition, we construct three model alloys based on P4/mmm space group symmetry, which is reduced to cubic P1 symmetry, by setting equal lattice parameter of a = 6.113 Å for all. The resulting structures simulated are: (AgSbTe2)2, Ag3SbTe4, and AgSb3Te4, which appear in Figure 1e, f, and g, respectively. All three structures contain 8 atoms per unit cell and Sb/Ag ratios of 1, 1/3, and 3, respectively. To calculate band structures of these three model alloys, spin-orbit (SO) magnetic calculations were performed utilizing a similar GGA/PAW routine as described above for uniform 7 × 7 × 7 Monkhorst-Pack
3.2. Experimental procedure
3.2.1. Materials synthesis
Experimental procedures implemented in this study are intended to validate the effects of La-alloying on TE performance, as predicted from first principles. They include synthesis of two model alloys, La-free and La-alloyed, having molar ratios (Ag:Sb:Te:La) of 18:29:53:0 and 15.75:29:53:2.25, respectively. Generally, synthesis procedures comprise vacuum melting and iced-water quenching, followed by uniaxial hot-pressing at two distinct temperatures, 540 and 500°C, yielding two series of 12.7 mm dia. pellets referenced below as Series A and Series B, respectively. The difference between these two series of alloys is manifested by their phase contents and average composition in matrix. These factors significantly affect TE performance, as will be discussed further below. A detailed description of the experimental procedures appears elsewhere .
3.2.2. Materials and thermoelectric property characterization
Materials characterization procedures include microstructure, phase identification, and composition analysis employing scanning electron microscopy and X-ray diffraction . Assessment of alloys’ thermal stability is investigated using SETARAM 1600 DSC with a scanning rate of 25 K min−1 at temperatures ranging from room temperature through 973 K.
Temperature-dependent electrical conductivity, σ(T), and Seebeck coefficient, S(T) (thermopower), of these pellets are measured in temperature range from 300 to ~700 K employing
4. Effects of La-alloying on thermoelectric performance
In this section, we introduce the concept resting behind La-alloying: its origin and implications, predictions from first principles, and experimental validations. Comparative discussion of the results in view of TE performance is provided.
4.1. Predictions from first-principles
4.1.1. The AgSbTe2(P4/mmm) phase
184.108.40.206. Structural and vibrational properties
P4/mmm form of AgSbTe2 phase is found to be the most stable one compared to all three polymorphs at temperatures larger than 400 K and exhibits Helmholtz free energy values with close proximity to those of cubic polymorph . Frequency-dependent v-DOS, , calculated for this compound applying Debye approximation exhibits two major peaks at ca. 2.0 and 2.7 THz, and discloses interesting feature. Whereas, 2.7 THz peak comprises equal contributions from lattice vibrations of all sublattice sites, 2.0 THz one is primarily ascribed to vibrations of Ag-sublattice site atoms [57, 58]. This opens up the option of tuning v-DOS pattern by introducing point defects, a discipline for which the term
Three substitutional options were tested, in which La substitutes for Ag, Sb, or Te, and it was found that substitution at Ag-sublattice sites is the most energetically preferred state for P4/mmm symmetry . Accordingly, La-doped structure was constructed, in which one La-atom substitutes for 1/8. of Ag-atoms, and is shown in Figure 1b. First, v-DOS was calculated for La-doped structure and 2.0 THz peak was suppressed, as expected. Second, phonon dispersion curves were calculated for both AgSbTe2 and LaAg7Sb8Te16 alloys close to Γ-point along c-crystallographic direction, indicating, that the slopes of the one longitudinal and two transverse acoustic modes of AgSbTe2-lattice are greater, than those of La-alloyed one . Quantitatively, average sound velocities derived for pure and La-alloyed materials are 1727 and 1046 m s−1, respectively. Moreover, temperature-dependent heat capacity functions were determined for both structures, yielding slightly lower values for La-alloyed material. Both values of sound velocity and heat capacity that are found to decrease due to La-alloying imply, that La-alloying should reduce lattice thermal conductivity . Additional calculations employing Debye approximation for low-temperature range of heat capacity yield Debye temperatures and sound velocities for both pure and La-alloyed materials, which are 112 K and 1684 m s−1 vs. 104 K and 1563 m s−1, respectively . It is noteworthy that evaluation of sound velocity in this manner is considered to be more physically reliable, since it represents the entire space of lattice directions, rather than individual one. It is, therefore, expected that this way of calculation should yield thermal conductivity values, that fit experimental data better than the former way does.
220.127.116.11. Effects of La-doping on thermal conductivity
Average sound velocity, , and Debye temperature, , evaluated from first-principles serve as input, that is required to evaluate lattice thermal conductivity, . To this end, one possibility is to employ Callaway model for lattice thermal conductivity [86, 87], which has become conventional, particularly in the field of TE materials [36–38, 88–93]. In present case, however, there is no need to employ Callaway model for several reasons. First, Callaway model is specified for low temperatures, where contributions of either Normal (N)- or Umklapp (U)-processes are at the same order of magnitude. For temperatures adequately higher than Debye temperature (e.g., ≈ 112 K for AgSbTe2 alloy) [30, 57], only U-processes dominate. Second, Callaway model considers and functions that are simplistically approximated based on Debye model . In present case, however, the explicit and functions have already been calculated for both pure and La-alloyed materials. Alternatively, the following expression for lattice thermal conductivity is employed [94–96]:
where is phonon relaxation time. To first approximation, it has been assumed that La-doping influences mostly sound velocity and heat capacity and has negligible effect on . The ratio of -products obtained for LaAg7Sb8Te16 andAgSbTe2 alloys, therefore, reflects the lower limit of relative reduction in thermal conductivity due to La-alloying. Applying dispersion curves close to Γ-point along c-crystallographic direction, it is predicted, that should decrease by factor of ca. 2.7 due to La-doping. Alternatively, applying sound velocity values derived from Debye approximation, is expected to decrease by ca. 14% at room temperature due to La-doping .
A more thorough and accurate treatment of expression (8) considers the effects of La-alloying on , as well. To evaluate
where is Grüneisen parameter that reflects the degree of lattice anharmonicity , and
To consider dependence of v-DOS on phonon frequency, frequency-averaged expression for is introduced, so that serves as weighting function:
where is Debye frequency. Equivalent relaxation time is then expressed as:
The resulting values of lattice thermal conductivity for LaAg7Sb8Te16 and AgSbTe2 alloys are obtained from Eq. (8) by substituting the respective physical magnitudes for both alloys in Eqs. (9)–(11) [19, 20, 30, 57, 58, 92] with ≈ 1 nm [5, 8, 16, 91]. Lattice thermal conductivity for LaAg7Sb8Te16 and AgSbTe2 alloys calculated as function of temperature appear in Figure 2.
It is shown that thermal conductivity exhibits realistic values, that correspond with data documented in the literature [19, 20, 25, 98] with marked decrease due to La-doping, ranging between relative values of 11 and 19%, depending on temperature.
18.104.22.168. Effects of La-doping on electrical properties
It was shown that La-alloying reduces lattice thermal conductivity values, which affects TE performance positively. To address, however, the total effects of La-alloying on TE performance, evaluation of electrical conductivity and Seebeck coefficient is essential. This goal was achieved from first-principles applying Boltzmann transport theory as described above for LaAg7Sb8Te16 and AgSbTe2 alloys. The results are plotted in Figure 3 in temperature range 50–1000 K.
It is found that La-doping results in reduction in electrical conductivity (e.g., from ca. 1800 down to 250 S cm−1 at room temperature) and, at the same time, increase in Seebeck coefficient, e.g., from ca. 4 up to 40 µV K−1 at room temperature. For the sake of comparison, Jovovic and Heremans reported on experimental measurements of electrical conductivity and Seebeck coefficients of stoichiometric and doped AgSbTe2 alloys at temperatures up to 400 K [19, 98]. For example, they report on electrical resistivity value of 5 × 10−5 Ohm m at 100 K for stoichiometric AgSbTe2 alloy, which is equivalent to 200 S cm−1.
They report also on electrical resistivity that increases with temperature, indicating charge carriers scattering. Additionally, electrical resistivity may either increase or decrease with doping, depending on dopant’s chemical identity. In the present case, electrical conductivity values are significantly larger, e.g., ca. 1900 S cm−1 at 100 K, and are decreasing with temperature, where La-doping reduces conductivity. Seebeck coefficient values reported by Jovovic et al. exhibit general trend of increase with temperature, which corresponds to trend calculated in the present case. Also, they report on general trend of increase in Seebeck coefficient values due to doping (except doping with AgTe), in agreement with the present study for La. Complementary trend is reported by Du et al. [25, 99]. Most interestingly, effects of La-doping on electrical properties of AgSbTe2 alloy are reported by Min et al. . They report on trends that are qualitatively similar to those of the present study. First, La-doping was also reported to reduce electrical conductivity, e.g., from ca. 400 S cm−1 for undoped AgSbTe2 down to 66 S cm−1 for 3 at.% La-doping at room temperature. Second, La-doping increases Seebeck coefficients, e.g., from ca. 90 µV·K−1 for undoped AgSbTe2 up to ca. 220 µV K−1 for 3 at.% La-doping at room temperature. Quantitatively, values of electrical conductivity calculated in this study are considered to be large with respect to the above cited studies. Conversely, Seebeck coefficient values calculated in this study are considered to be smaller than those reported by the above studies. We note, however, that such calculations are most meaningful for comparative purposes, since they rest upon values, that should be calibrated against experimental data, such as electronic chemical potential and relaxation times.
It is indicated that the effects of La-doping on electrical conductivity and Seebeck coefficient are opposite to each other. Evaluation of TE power factor (PF; ) is, therefore, necessary in order to realize how La affects TE power conversion. Figure 4 displays PF calculated for LaAg7Sb8Te16 and AgSbTe2 alloys in temperature range 50–1000 K.
It is shown that La-doping has considerably positive effect on PF. This also corresponds with the data reported by Min et al. , specifically for low La-concentration regime. We note that, moreover, La-doping reduces lattice thermal conductivity, as shown in Figure 2. We conclude that La-alloying should improve energy conversion efficiency of AgSbTe2 (P4/mmm), as reflected by increased TE figure-of-merit.
4.1.2. Formation of Sb2Te3 and Sb8Te3(R-3m) phases
The single δ-phase is Sb-rich phase based on AgSbTe2 alloy. Since it has limited solubility to Sb with relatively moderate slope of Sb-solvus, it is likely to decompose to δ+Sb2Te3 phase mixture [28, 29, 100–103], whereas Sb2Te3 is equilibrium phase and may appear as different homologous forms [72, 73, 104–107]. Precipitation of antimony-telluride second phase in δ-matrix is expected to affect TE performance due to contributions from both matrix and precipitate phases or variation of the average matrix composition. In the following sections, we address both aspects. Section 22.214.171.124 introduces the issue of precipitation sequence based on bulk/interfacial energetic considerations, and Section 126.96.36.199 predicts the effects of phase formation on electronic properties. Then, Section 4.1.3 deals with compositional variations in the matrix and their effects on electronic properties.
188.8.131.52. The precipitation sequence: energetic aspects
Nucleation of Sb2Te3 and Sb8Te3 phases from Sb-saturated δ-AgSbTe2 matrix has been observed, which can be associated to different experimental conditions. To account for the sequence of phase formation, information on both bulk and interfacial energetics is required. The formation energies of Sb2Te3 and Sb8Te3 (R-3m) phases, calculated according to Eq. (5), are −62 and −56.6 kJ mol−1, respectively. This implies that Sb2Te3 is more energetically favorable, assuming, that Sb2Te3 precipitates are adequately large, so that, interfaces do not play significant role. To address the role of interfaces, free energies of Sb2Te3/AgSbTe2 and Sb8Te3/AgSbTe2 interfaces are evaluated. To this end, two slab models of (Sb2Te3)2/(AgSbTe2)5/(Sb2Te3)2 (40 atoms) and (AgSbTe2)3/(Sb8Te3)6/(AgSbTe2)3 (90 atoms) forms are constructed, respectively, consisting of two interfaces each, exhibiting and orientation relationship, which was observed experimentally . Both structures are displayed in Figure 5.
It is noted that two interfaces presented in both slabs shown in Figure 5a and b consist of different Sb- and Te-terminating planes, so that interfacial free energies calculated according to Eq. (6) represent an average value for both terminations. Correction factor is, therefore, applied to represent interfacial free energy of low-energy Sb-termination. The resulting values for Sb2Te3/AgSbTe2 and Sb8Te3/AgSbTe2 interfaces are = 208 and 175 mJ m−2, respectively. These values are considered to be relatively low compared to those of intermetallic compounds and are comparable with those of pure metals . This is, however, not surprising, considering the extremely small atomic misfit between the and crystallographic planes , which encourages formation of Sb2Te3 or Sb8Te3 precipitates in the form of long lamellae along these planes [28, 29, 57, 58, 100–103]. These low values of interfacial free energy also initiate fast nucleation, thanks to low activation energy for nucleation, which is proportional to .
Interestingly, Sb2Te3 phase exhibits lower value of formation energy and higher value of interfacial free energy compared to those of Sb8Te3 phase. This implies that Sb8Te3 is metastable phase that may form prior to the nucleation of Sb2Te3 equilibrium phase [28, 29, 100–103]. Suggested nucleation sequence is, therefore, supersaturated-δ → supersaturated-δ + Sb8Te3 → equilibrium-δ + Sb2Te3.
184.108.40.206. Effects of Sb2Te3 and Sb8Te3 formation on electronic properties
In view of aforementioned prospect for the presence of either of Sb2Te3- or Sb8Te3-phases in AgSbTe2-matrix, calculations of transport coefficients of these phases provide us with predictions of the effects such phase mixture on TE performance. Figure 6 displays electrical conductivity and Seebeck coefficients calculated in temperature range 50–1000 K.
It is shown that both electrical conductivity and Seebeck coefficient values of Sb2Te3 phase are larger than those of Sb8Te3 phase in wide temperature range, e.g., ca. 2100 S cm−1 and 85 µV K−1 for Sb2Te3 compared to 1380 S cm−1 and 29 µV K−1 for Sb8Te3 at 300 K, respectively. Moreover, comparison of these results with the data shown in Figure 3 for AgSbTe2-matrix implies that precipitation of Sb2Te3 phase yields positive influence on TE performance: both electrical conductivity and Seebeck coefficient increase. It is strikingly indicated that the effects of Sb2Te3 precipitation are even greater, than those of La-doping. It is, therefore, concluded that the desirable material from TE viewpoint is La-doped, Sb-supersaturated δ-AgSbTe2-matrix that is aged for a certain duration to form considerable amount of Sb2Te3 phase. The effects of Sb8Te3 phase on TE performance are, conversely, inferior to those of Sb2Te3 phase. Sb8Te3 is, however, metastable phase and is not expected to prevail for long durations at elevated temperatures (e.g., under service conditions of TE generator) due to low thermal stability.
4.1.3. Effects of off-stoichiometry on electronic properties of the AgSbTe2 phase
An additional effect taking place during precipitation of any SbpTeq phase from Sb-supersaturated δ-matrix is enrichment of δ-matrix with Ag-atoms and depletion of Sb. To simulate these compositional variations, two off-stoichiometric model alloys are constructed, namely Ag3SbTe4 and AgSb3Te4, in addition to stoichiometric AgSbTe2 phase. These model compounds, appearing in Figure 1e, g, and f, exhibit Sb/Ag ratios of 1/3, 3, and 1, respectively. Figure 7 displays electrical conductivity and Seebeck coefficient values calculated in temperature range 50–1000 K.
It is shown, that increase in Sb/Ag ratio results in decrease in electrical conductivity simultaneously with increase in Seebeck coefficient. This trend corresponds well with study of Jovovic and Heremans , who reported on decrease in both Seebeck coefficient and electrical resistivity due to additions of 2% AgTe to stoichiometric AgSbTe2-phase, i.e., reducing Sb/Ag ratio. It should be noted that comparison of this trend with data reported in the literature is not straightforward, since compositional changes involve in practice not only Sb/Ag ratio, but also ratio of Te to any of the other species. Additionally, deviations from given stoichiometry often involve formation of second phases, which is not directly simulated here. For instance, Zhang et al. reported on dependence of TE properties on composition for Ag2−ySbyTe1+y -based alloys and found that electrical conductivity increases, while Seebeck coefficient decreases with
Most importantly, this predicted effect of Sb/Ag ratio on electrical properties has major implications on the temporal evolution of TE performance of the material during aging heat treatments (below Sb-solvus), or of TE generator during service. Since SbpTeq phases nucleate from Sb-supersaturated δ-matrix during heat treatments, Sb/Ag ratio in δ-matrix decreases. This should be accompanied by increase in electrical conductivity concurrently with decrease in Seebeck coefficient.
5. Experimental results
It was shown above how first-principles calculations provide us with information about all aspects concerning TE transport behavior, including thermal and electrical conductivity and Seebeck coefficient. Most importantly, this assists us in tailoring the material by introducing lattice defects to enhance its TE performance. In the following section, we introduce experimental procedures taken for validating the above predictions. Comparing between both aspects is, moreover, very instructive not only on engineering aspects, but also on universal aspect, by realizing how to implement computational tools to predict properties of other materials.
5.1. Microstructure and implications on thermoelectric behavior
As mentioned above, two classes of La-alloyed AgSbTe2-based materials were prepared by uniaxial hot-pressing at 540 or 500°C, and are classified as Series A and Series B, respectively. The ideal case for testing the effects of La-doping is single δ-phase dissolving La homogeneously. This, however, is difficult to achieve. Hot-pressing at 540°C, that is, above Sb-solvus, expected to yield the desirable single δ-phase that does not contain Sb2Te3 precipitates [101–103]. These Sb2Te3 precipitates, indeed, were not observed in Series A samples; however, La-rich precipitates having stoichiometry close to LaTe2 were observed . As a result, δ-matrix was found to be depleted of La , which does not allow us comparison between La-free and La-doped samples. Conversely, samples of Series B, that were hot-pressed at 500°C, exhibit considerable amount of Sb2Te3 phase, which is expected; however, LaTe2 precipitates are dissolved, so that δ-matrix contains adequately large amount of La, close to its nominal concentration. Series B is, therefore, more suitable to exemplify the effects of La-doping. Moreover, as predicted from first-principles, the presence of Sb2Te3 precipitates, in addition to La solute atoms, has positive effects on electronic transport.
5.2. Thermal analysis
Thermal conductivity measurements performed for both Series A and Series B indicate the expected trend. First, all thermal conductivity values lie in the range 0.6–0.8 W m−1 K−1 . Second, samples of Series A did not exhibit any considerable difference between La-free and La-doped materials . This is associated to depletion of δ-matrix from La solute atoms, so that, matrix composition of La-doped and La-free materials is practically the same. Third, and most importantly, it was found that thermal conductivity of La-doped materials is significantly lower than those of La-free materials of Series B, e.g., 0.8 W m−1 K−1 for La-free and 0.6 W m−1 K−1 for La-doped samples at 500 K. This is strikingly corroborated by predictions from first-principles, both qualitatively and quantitatively, as shown in Figure 2. It is also noteworthy that both values coincide at temperatures larger than 650 K, which can be associated with phase transition [58, 101–103]. Thorough discussion of thermal conductivity values measured for Series A and Series B materials and their relationship with microstructure appears elsewhere . To address this issue of phase transition, DSC measurements were implemented for both La-free and La-doped samples, Figure 8.
Endothermic peak at around 630–650 K is observed for La-free material, which is associated with Ag2Te + Sb2Te3 → δ-AgSbTe2 phase transition at 360°C [101–103]. La-doped material, however, does not exhibit this transition. This corresponds well with thermal conductivity behavior reported by us earlier , in which temperature-dependent thermal conductivity of La-doped materials show up continuous trend, whereas La-free materials exhibit sharp drop of thermal conductivity around this temperature. This implies that La-additions help in stabilizing δ-phase against decomposition, which is expected to contribute to stability of TE device operation at service conditions. Sharp endothermic peak at ca. 860 K, which is common for both La-free and La-doped materials, is associated to melting.
5.3. Electrical property measurements
It was predicted from first-principles that La-doping reduces electrical conductivity and increases Seebeck coefficient, Figure 3. Measurements of electrical conductivity and Seebeck coefficients were carried out for both Series A and Series B materials. The samples of Series B are of our interest, since they dissolve La-atoms in δ-matrix; we will, therefore, introduce these results first. Figure 9 displays experimentally collected electrical conductivity and Seebeck coefficient values of La-free and La-doped materials of Series B.
It is shown that electrical conductivity values decrease, e.g., from ca. 1400 down to 900 S cm−1 at room temperature, and Seebeck coefficient increase, e.g., from ca. 30 up to 70 µV K−1 at room temperature, due to La-doping. This behavior is, qualitatively, the same as that observed for calculated values shown in Figure 3. Moreover, temperature dependence, that is, electrical conductivity decreasing and Seebeck coefficient increasing with temperature for both La-free and La-doped materials, is identical to that indicated by calculated values shown in Figure 3. There are two major differences between experimental and calculated values appearing in Figures 3 and 9, respectively. First, the absolute values of measured Seebeck coefficient values are greater than calculated ones. Also, difference of electrical conductivity between La-doped and La-free materials is smaller for measured dataset than for calculated ones. This is probably due to difficulty to simulate low dopant concentrations in DFT . Second, it is noteworthy that both values of electrical conductivity and Seebeck coefficients measured for La-free and La-doped materials converge at temperatures >650 K, Figure 9. Interestingly, these convergences occur due to sharp deviations of the values featured by La-free material, whereas the values of La-doped materials preserve their continuous trendline. This observation corresponds well with the behavior shown by DSC curves in Figure 8, where La-free compound decomposes at around 650 K, whereas La-doped compound seem to preserve its thermal stability. This also corresponds with converging thermal conductivities of the samples of Series B as discussed above . Following our comparative discussion in Section 220.127.116.11, experimental values of electrical properties are found to be closer to experimental values reported in the literature than to calculated values [19, 25, 27, 98, 99].
To complement our understanding of the effects of La-doping on electronic properties, we measured temperature-dependent electrical conductivity and Seebeck coefficient values for the samples of Series A, as well. The results are plotted against temperature in Figure 10.
Comparison between the results attained for alloys of Series A and Series B is very instructive. As noted, the samples of Series A exhibited formation of LaTe2-like precipitates, which “drain out” La atoms from δ-matrix, resulting in matrix compositions, that are nearly identical to each other for La-free and La-doped materials. For this reason, thermal conductivity values measured for La-free and La-doped materials seem to be practically identical in wide temperature range . It is, therefore, not surprising to observe the same behavior for electrical properties, Figure 10.
It is indicated, that both electrical conductivity and Seebeck coefficient values measured for La-free and La-doped materials seem to be very close to each other in the entire temperature range, probably due to nearly identical matrix compositions for La-free and La-doped materials. Additionally, electrical conductivity and Seebeck coefficients featured by La-doped alloys exhibit relatively continuous temperature-dependent behavior, whereas values, measured for La-free alloys exhibit curled behavior. This, again, can be explained in terms of poor thermal stability of La-free materials, as discussed above.
5.4. Implications for thermoelectric power conversion
It has been shown that La-doping has unequivocally positive effect on reducing lattice thermal conductivity, both computationally and experimentally. The effects on electrical properties, particularly electrical conductivity and Seebeck coefficient, are opposing each other. To assess the effects of La-doping on device’s power capacity, TE PFs of La-free and La-doped materials of Series B are evaluated based on the data displayed in Figure 9. The results are shown in Figure 11.
It is clearly shown that La-doping affects positively PF for temperatures lower than 500 K, e.g., PF determined for room temperature increases from ca. 200 to 400 µW m−1 K−2 due to La-doping. At higher temperatures, PFs of La-free and La-doped materials are practically identical. The maximum PF values observed are around 1000 µW m−1 K−2. This trend is similar to that reported by Min et al. , that is, PF increasing from 300 up to 1500 µW m−1 K−2 in respective temperature range from room temperature to 400°C for AgSbTe2 alloy.
La-doping was tested by them for different compositions, where composition yielding the greatest PF values is AgSb0.99La0.01Te2, with PF values around 1000–1200 µW m−1 K−2 in the entire temperature range. Particularly, this La-doped material exhibits superior PF values up to ca. 325°C. This trend is similar to that reported by us in this study.
Finally, determination of TE figure-of-merit for both La-free and La-doped materials will provide us with the ultimate indication whether La-doping enhances TE power conversion efficiency. Based on thermal and electrical properties measured for Series A and Series B, temperature-dependent
Most importantly, it is shown that La-doping increases
The picture, revealed for alloys of Series A, is, however, different; it is shown in Figure 12a that La-doping has little or no effect on
6. Summary and concluding remarks
This chapter introduced the following findings. Computationally, total energy calculations for different polymorphs of AgSbTe2 phase yield their Helmholtz free energies, implying, that P4/mmm space group symmetry is the most stable one at temperatures adequately higher than room temperatures. Predictions of the effects of doping on thermal conductivity are established on calculations of vibrational properties, such as phonon dispersion and density of states, from first-principles. Based on specific features in v-DOS curve, it is hypothesized that La-substitution for Ag-sites should result in reduced lattice thermal conductivity. These calculations predict reduction in average sound velocity from 1684 to 1563 m s−1 and of Debye temperature from 112 to 104 K due to La-doping. Applying Umklapp mechanism for phonon scattering with frequency-averaged inverse relaxation time, which is combined with boundary scattering, yields temperature-dependent functional forms for lattice thermal conductivity. Marked decrease due to La-doping, ranging between relative values of 11 and 19% depending on temperature, are observed. Then, calculations of electronic band structures of both La-free and La-doped lattices are performed, yielding TE transport coefficients applying Boltzmann transport theory. It is found that La-doping results in reduction in electrical conductivity (e.g., from ca. 1800 down to 250 S cm−1 at room temperature) at the same time with increase in Seebeck coefficient, e.g., from ca. 5 up to 40 µV K−1 at room temperature.
Attempts to infer conclusions with practical implications from DFT calculations must consider engineering aspects that extend further beyond single phase state having high symmetry unit cell, that maintains its physical properties with time. For example, considerations, such as long-term device operation under elevated service temperatures, should be taken into account. Such case requires original solution for simplified (or, sometimes, over-simplified) approach offered by DFT. Particularly, for the case of thermal stability, exposure of Sb-rich δ-phase to elevated temperatures results in precipitation of SbpTeq-based phases at the same time with decrease in Sb/Ag ratio in δ-matrix. In this manner, thermal stability issues can be addressed by dividing the realistic conditions into a set of simplified problems, each can be handled by DFT. To this end, we first consider the case in which Sb2Te3 and Sb8Te3 phases precipitate inside AgSbTe2-matrix. It is found that both electrical conductivity and Seebeck coefficient values of Sb2Te3-phase are larger, than those of Sb8Te3-phase in wide temperature range, e.g., ca. 2100 S cm−1 and 85 µV K−1 for Sb2Te3 compared to1380 S cm−1 and 29 µV K−1 for Sb8Te3 at 300 K, respectively. Moreover, it is estimated that precipitation of Sb2Te3-phase in AgSbTe2-matrix is expected to improve the total values of both electrical conductivity and Seebeck coefficient. Concerning nucleation sequence of Sb2Te3 and Sb8Te3 phases in AgSbTe2, their molar formation energies and interfacial free energies were calculated, suggesting that Sb8Te3 nucleates first as metastable phase, prior to the formation of equilibrium Sb2Te3 phase. Second, to address the influence of deviations from AgSbTe2 stoichiometry on electron transport properties, off-stoichiometric model alloys Ag3SbTe4 and AgSb3Te4 were simulated. It is found that increase in Sb/Ag ratio results in decrease in electrical conductivity simultaneously with increase in Seebeck coefficient. Considering both effects of Sb2Te3 precipitation accompanied by simultaneous decrease in Sb/Ag ratio in δ-matrix taking place with aging time at temperatures below δ-solvus, it is expected that electrical conductivity of two-phase δ+Sb2Te3 alloy should increase with aging time, disregarding effects, such as electron boundary scattering. Interestingly, these two effects have opposite consequences regarding Seebeck coefficient, so that, it is difficult to assess resulting Seebeck coefficient.
Experimentally, model ternary (AgSbTe2) and quaternary (3 at.% La-AgSbTe2) alloys were synthesized by vacuum melting followed by quenching and hot-pressing. The appropriate conditions enabling formation of AgSbTe2-matrix that dissolves La-atoms with no La-rich precipitates were established. DSC tests enable observation of Ag2Te+Sb2Te3→δ-AgSbTe2 phase transition at 360°C for La-free alloys only, indicating improvement of alloy’s thermal stability due to La-additions. Temperature-dependent thermal conductivity of both alloys indicate reduction in thermal conductivity as a result of La-alloying from 0.92 to 0.71 W m−1 K−1 at 573 K, which corresponds with the trend predicted from first-principles. Measurements of temperature-dependent electrical conductivity and Seebeck coefficients indicate that La-doping reduces electrical conductivity and increases Seebeck coefficients, as predicted from first-principles. Eventually, it is shown that La-doping has positive effects on TE figure-of-merit
We demonstrate how first-principles calculations serve as trustworthy tool for predicting TE performance of materials, screening the best candidates for application in TE devices. It is noteworthy that such DFT routines prove to be very efficient by prediction of TE properties in a way saving expensive and time-consuming experiments. The resulting materials that seem to possess improved performance are, eventually, processed in laboratory. We show how simple physical considerations can be implemented in DFT calculations and lead to improvement of power conversion efficiency. La-doping improves the alloys’ thermal stability and reduces their thermal conductivity, as well as enhances TE power factor in certain temperature range. As a result, the total TE figure-of-merit improves significantly. We, finally, emphasize the universal aspects of this approach that can be applied for other TE materials, as well.
The author wishes to acknowledge generous support from the Israel Science Foundation (ISF), Grant no. 698/13, as well as, from the German-Israeli Foundation for Research and Development (GIF), Grant no. I-2333-1150.10/2012. Partial support from the Nancy and Stephen Grand Technion Energy Program (GTEP), the Russell Berrie Nanotechnology Institute (RBNI), Technion, and the Adelis Foundation for renewable energy research are greatly acknowledged, as well.
Martin RM.: Electronic Structure – Basic Theory and Practical Methods. Cambridge, UK: Cambridge University Press; 2004.
Argaman N, Makov G.: Density functional theory: An introduction. Am. J. Phys. 2000; 68:69–79. doi:10.1119/1.19375
Mishin Y, Asta M, Li J.: Atomistic modeling of interfaces and their impact on microstructure and properties. Acta. Mater. 2010; 58:1117–51. doi:10.1016/j.actamat.2009.10.049
Parr RG, Yang W.: Density-Functional Theory of Atoms and Molecules. New York: Oxford University Press; 1989.
Hsu KF, Loo S, Guo F, Chen W, Dyck JS, Uher C, Hogan T, Polychroniadis EK, Kanatzidis MG.: Cubic AgPbmSbTe2+m: bulk thermoelectric materials with high figure of merit. Science. 2004; 303:818–821. doi:10.1126/science.1092963
Kanatzidis MG.: Nanostructured thermoelectrics: The new paradigm? Chem. Mater. 2010; 22:648–659. doi:10.1021/cm902195j
Dadda J, Muller E, Klobes B, Pereira PB, Hermann R.: Electronic properties as a function of Ag/Sb ratio in Ag1-yPb18Sb1+zTe20 compounds. J. Electron. Mater. 2012; 41:2065–72. doi:10.1007/s11664-012-2111-9
Dadda J, Muller E, Perlt S, Hoche T, Pereira PB, Hermann RP.: Microstructures and nanostructures in long-term annealed AgPb18SbTe20 (LAST-18) compounds and their influence on the thermoelectric properties. J. Mater. Res. 2011; 26:1800–1812. doi:10.1557/jmr.2011.142
Perlt S, Hoche T, Dadda J, Muller E, Pereira PB, Hermann R, Sarahan M, Pippel E, Brydson R.: Microstructure analyses and thermoelectric properties of Ag1-xPb18Sb1+yTe20. J. Solid State Chem. 2012; 193:58–63. doi:10.1016/j.jssc.2012.03.064
Cook BA, Kramer MJ, Harringa JL, Han MK, Chung DY, Kanatzidis MG.: Analysis of nanostructuring in high figure-of-merit Ag1-xPbmSbTe2+m thermoelectric materials. Adv. Funct. Mater. 2009; 19:1254–1259. doi:10.1002/adfm.200801284
Sootsman JR, Chung DY, Kanatzidis MG.: New and old concepts in thermoelectric materials. Angew. Chem-Int. Edit. 2009; 48:8616–8639. doi:10.1002/anie.200900598
Steimer C, Welnic W, Kalb J, Wuttig M.: Towards an atomistic understanding of phase change materials. J. Optoelectron. Adv. Mater. 2006; 8:2044–2050.
Wang K, Steimer C, Detemple R, Wamwangi D, Wuttig M.: Assessment of Se based phase change alloy as a candidate for non-volatile electronic memory applications. Appl. Phys. A. 2005; 81:1601–1605. doi:10.1007/s00339-005-3358-2
Siegert KS, Lange FRL, Sittner ER, Volker H, Schlockermann C, Siegrist T, Wuttig M.: Impact of vacancy ordering on thermal transport in crystalline phase-change materials. Rep. Prog. Phys. 2015; 78:013001. doi:10.1088/0034-4885/78/1/013001
Wuttig M, Yamada N.: Phase-change materials for rewriteable data storage. Nat. Mater. 2007; 6:1004. doi:10.1038/nmat2077
Ma J, Delaire O, May AF, Carlton CE, McGuire MA, VanBebber LH, Abernathy DL, Ehlers G, Hong T, Huq A, Tian W, Keppens VM, Shao Horn Y, Sales BC.: Glass-like phonon scattering from a spontaneous nanostructure in AgSbTe2. Nat. Nano. 2013; 8:445–451. doi:10.1038/nnano.2013.95
Specht ED, Ma J, Delaire O, Budai JD, May AF, Karapetrova EA.: Nanoscale structure in AgSbTe2 determined by diffuse elastic neutron scattering. J. Electron. Mater. 2015; 44:1536–9. doi:10.1007/s11664-014-3447-0
Shinya H, Masago A, Fukushima T, Katayama-Yoshida H.: Inherent instability by antibonding coupling in AgSbTe2. Jpn. J. Appl. Phys. 2016; 55:6. doi:10.7567/jjap.55.041801
Jovovic V, Heremans JP.: Doping effects on the thermoelectric properties of AgSbTe2. J. Electron. Mater. 2009; 38:1504–1509. doi:10.1007/s11664-009-0669-7
Morelli DT, Jovovic V, Heremans JP.: Intrinsically minimal thermal conductivity in cubic I-V-VI2 semiconductors. Phys. Rev. Lett. 2008; 101:035901. doi:10.1103/PhysRevLett.101.035901
Nielsen MD, Ozolins V, Heremans JP.: Lone pair electrons minimize lattice thermal conductivity. Energy Environ. Sci. 2013; 6:570–578. doi:10.1039/C2EE23391F
Ye L-H, Hoang K, Freeman AJ, Mahanti SD, He J, Tritt TM, Kanatzidis MG.: First-principles study of the electronic, optical, and lattice vibrational properties of AgSbTe2. Phys. Rev. B. 2008; 77:245203. doi:10.1103/PhysRevB.77.245203
Lencer D, Salinga M, Grabowski B, Hickel T, Neugebauer J, Wuttig M.: A map for phase-change materials. Nat. Mater. 2008; 7:972–977. http://www.nature.com/nmat/journal/v7/n12/suppinfo/nmat2330_S1.html
Shportko K, Kremers S, Woda M, Lencer D, Robertson J, Wuttig M.: Resonant bonding in crystalline phase-change materials. Nat. Mater. 2008; 7:653–658. doi:10.1038/nmat2226
Du B, Li H, Xu J, Tang X, Uher C.: Enhanced figure-of-merit in Se-doped p-type AgSbTe2 thermoelectric compound. Chem. Mater. 2010; 22:5521–5527. doi:10.1021/cm101503y
Ma H, Su T, Zhu P, Guo J, Jia X.: Preparation and transport properties of AgSbTe2 by high-pressure and high-temperature. J. Alloys Compd. 2008; 454:415–418. doi:10.1016/j.jallcom.2006.12.126
Min BK, Kim BS, Kim IH, Lee JK, Kim MH, Oh MW, Park SD, Lee HW.: Electron transport properties of La-doped AgSbTe2 thermoelectric compounds. Electron. Mater. Lett. 2011; 7:255–260. doi:10.1007/s13391-011-0914-0
Sharma PA, Sugar JD, Medlin DL.: Influence of nanostructuring and heterogeneous nucleation on the thermoelectric figure of merit in AgSbTe2. J. Appl. Phys. 2010; 107:113716. doi:10.1063/1.3446094
Sugar JD, Medlin DL.: Precipitation of Ag2Te in the thermoelectric material AgSbTe2. J. Alloys Compd. 2009; 478:75–82. doi:10.1016/j.jallcom.2008.11.054
Pereira PB. Structure and Lattice Dynamics of Thermoelectric Complex Chalcogenides. Julich Forschungszentrum: Universite de Liege; 2012.
Barabash SV, Ozolins V, Wolverton C.: First-principles theory of competing order types, phase separation, and phonon spectra in thermoelectric AgPbmSbTem+2 alloys. Phys. Rev. Lett. 2008; 101:155704. doi:10.1103/PhysRevLett.101.155704
Hoang K, Mahanti SD, Salvador JR, Kanatzidis MG.: Atomic ordering and gap formation in Ag-Sb-based ternary chalcogenides. Phys. Rev. Lett. 2007; 99:156403.doi:10.1103/PhysRevLett.99.156403
Rezaei N, Hashemifar SJ, Akbarzadeh H.: Thermoelectric properties of AgSbTe2 from first-principles calculations. J. Appl. Phys. 2014; 116:103705. doi:10.1063/1.4895062
Singh DJ, Terasaki I.: Thermoelectrics - nanostructuring and more. Nat. Mater. 2008; 7:616–617. doi:10.1038/nmat2243
Toberer ES, Zevalkink A, Snyder GJ.: Phonon engineering through crystal chemistry. J. Mater. Chem. 2011; 21:15843–15852. doi:10.1039/c1jm11754h
He JQ, Girard SN, Kanatzidis MG, Dravid VP.: Microstructure-lattice thermal conductivity correlation in nanostructured PbTe0.7S0.3 thermoelectric materials. Adv. Funct. Mater. 2010; 20:764–772. doi:10.1002/adfm.200901905
He JQ, Sootsman JR, Girard SN, Zheng JC, Wen JG, Zhu YM, Kanatzidis MG, Dravid VP.: On the origin of increased phonon scattering in nanostructured PbTe based thermoelectric materials. J. Am. Chem. Soc. 2010; 132:8669–8675. doi:10.1021/ja1010948
Kim W, Singer SL, Majumdar A, Zide JMO, Klenov D, Gossard AC, Stemmer S.: Reducing thermal conductivity of crystalline solids at high temperature using embedded nanostructures. Nano Lett. 2008; 8:2097–2099. doi:10.1021/nl080189t
Du B, Li H, Tang X.: Effect of Ce substitution for Sb on the thermoelectric properties of AgSbTe2 compound. J. Electron. Mater. 2014; 43:2384–2389. doi:10.1007/s11664-014-3076-7
Du BL, Li H, Tang XF.: Enhanced thermoelectric performance in Na/Se doped p-type AgSbTe2 compound. J. Inorg. Mater. 2011; 26:680–684. doi:10.3724/sp.j.1077.2011.00680
Du BL, Li H, Tang XF.: Enhanced thermoelectric performance in Na-doped p-type nonstoichiometric AgSbTe2 compound. J. Alloys Compd. 2011; 509:2039–2043. doi:10.1016/j.jallcom.2010.10.131
Mohanraman R, Sankar R, Boopathi KM, Chou FC, Chu CW, Lee CH, Chen Y-Y.: Influence of In doping on the thermoelectric properties of an AgSbTe2 compound with enhanced figure of merit. J. Mater. Chem A. 2014; 2:2839–2844. doi: 10.1039/c3ta14547f
Mohanraman R, Sankar R, Chou FC, Lee CH, Chen Y-Y.: Enhanced thermoelectric performance in Bi-doped p-type AgSbTe2 compounds. J. Appl. Phys. 2013; 114. doi:10.1063/1.4828478
Wu H-j, Chen S-w, Ikeda T, Snyder GJ.: Reduced thermal conductivity in Pb-alloyed AgSbTe2 thermoelectric materials. Acta Mater. 2012; 60:6144–6151. doi:10.1016/j.actamat.2012.07.057
Zhang H, Luo J, Zhu HT, Liu QL, Liang JK, Li JB, Liu GY.: Synthesis and thermoelectric properties of Mn-doped AgSbTe2 compounds. Chin. Phys. B. 2012; 21:6. doi:10.1088/1674-1056/21/10/106101
Zhang H, Luo J, Zhu HT, Liu QL, Liang JK, Rao GH.: Phase stability, crystal structure and thermoelectric properties of Cu doped AgSbTe2. Acta Phys. Sin. 2012; 61:7.
Zhang SN, Jiang GY, Zhu TJ, Zhao XB, Yang SH.: Doping effect on thermoelectric properties of nonstoichiometric AgSbTe2 compounds. Int. J. Miner. Metall. Mater. 2011; 18:352–356. doi:10.1007/s12613-011-0446-5
Mohanraman R, Sankar R, Chou F-C, Lee C-H, Iizuka Y, Muthuselvam IP, Chen Y-Y: Influence of nanoscale Ag2Te precipitates on the thermoelectric properties of the Sn doped P-type AgSbTe2 compound. APL Mater. 2014; 2:096114. doi:10.1063/1.4896435
Du B, Xu J, Zhang W, Tang X.: Impact of in situ generated Ag2Te nanoparticles on the microstructure and thermoelectric properties of AgSbTe2 compounds. J. Electron. Mater. 2011; 40:1249–53. doi:10.1007/s11664-011-1620-2
Zhang SN, Zhu TJ, Yang SH, Yu C, Zhao XB.: Improved thermoelectric properties of AgSbTe2 based compounds with nanoscale Ag2Te in situ precipitates. J. Alloys Compd. 2010; 499:215–220. doi:10.1016/j.jallcom.2010.03.170
Du B, Yan Y, Tang X.: Variable-temperature in situ X-ray diffraction study of the thermodynamic evolution of AgSbTe2 thermoelectric compound. J. Electron. Mater. 2015; 44:2118–2123. doi:10.1007/s11664-015-3682-z
Li HY, Jing HY, Han YD, Lu GQ, Xu LY, Liu T.: Interfacial evolution behavior of AgSbTe2.01/nanosilver/Cu thermoelectric joints. Mater. Des. 2016; 89:604–610. doi:10.1016/j.matdes.2015.09.163
Wyzga PM, Wojciechowski KT.: Analysis of the influence of thermal treatment on the stability of Ag1−xSb1+xTe2+x and Se-doped AgSbTe2. J. Electron. Mater. 2016; 45:1548–1554. doi:10.1007/s11664-015-4102-0
Pei Y, Lensch-Falk J, Toberer ES, Medlin DL, Snyder GJ.: High thermoelectric performance in PbTe due to large nanoscale Ag2Te precipitates and La doping. Adv. Funct. Mater. 2011; 21:241–249. doi:10.1002/adfm.201000878
Takagiwa Y, Pei Y, Pomrehn G, Snyder GJ.: Dopants effect on the band structure of PbTe thermoelectric material. Appl. Phys. Lett. 2012; 101:092102–3. doi:10.1063/1.4748363
Min B-K, Kim B-S, Oh M-W, Ryu B-K, Lee J-E, Joo S-J, Park S-D, Lee H-W, Lee H-s.: Effect of La-doping on AgSbTe2 thermoelectric compounds. J. Korean Phys. Soc. 2016; 68:164–169. doi:10.3938/jkps.68.164
Amouyal Y.: On the role of lanthanum substitution defects in reducing lattice thermal conductivity of the AgSbTe2 (P4/mmm) thermoelectric compound for energy conversion applications. Comput. Mater. Sci. 2013; 78:98–103.doi:10.1016/j.commatsci.2013.05.027
Amouyal Y.: Reducing lattice thermal conductivity of the thermoelectric compound AgSbTe2 (P4/mmm) by lanthanum substitution: computational and experimental approaches. J. Electron. Mater. 2014; 43:3772–3779. doi:10.1007/s11664-014-3145-y
Quarez E, Hsu KF, Pcionek R, Frangis N, Polychroniadis EK, Kanatzidis MG.: Nanostructuring, compositional fluctuations, and atomic ordering in the thermoelectric materials AgPbmSbTe2+m. The myth of solid solutions. J. Am. Chem. Soc. 2005; 127:9177–9190. doi:10.1021/ja051653o
Kresse G, Furthmuller J.: Efficiency of ab-initio total energy calculations for metals and semiconductors using a plane-wave basis set. Comput. Mater. Sci. 1996; 6:15–50. doi:10.1016/0927-0256(96)00008-0
Kresse G, Furthmueller J.: Efficient iterative schemes for Ab Initio total-energy calculations using a plane-wave basis set. Phys. Rev. B: Condens. Matter Mater. Phys. 1996; 54:11169–11186. doi:10.1103/PhysRevB.54.11169
Kresse G, Hafner J.: Ab initio molecular-dynamics simulation of the liquid-metal-amorphous-semiconductor transition in Germanium. Phys. Rev. B: Condens. Matter Mater. Phys. 1994; 49:14251–14269. doi:10.1103/PhysRevB.49.14251
MedeA®: Materials Design, Inc. 2010;v. 2.74. Angel Fire, NM, USA.
Perdew JP, Ruzsinszky A, Csonka GI, Vydrov OA, Scuseria GE, Constantin LA, Zhou X, Burke K.: Restoring the density-gradient expansion for exchange in solids and surfaces. Phys. Rev. Lett. 2008; 100:136406. doi:10.1103/PhysRevLett.100.136406
Kresse G, Joubert D.: From ultrasoft pseudopotentials to the projector augmented-wave method. Phys. Rev. B. 1999; 59:1758. doi:10.1103/PhysRevB.59.1758
Blöchl PE, Jepsen O, Andersen OK.: Improved tetrahedron method for Brillouin-zone integrations. Phys. Rev. B. 1994; 49:16223–16233. doi:10.1103/PhysRevB.49.16223
Madsen GKH, Singh DJ.: BoltzTraP. A code for calculating band-structure dependent quantities. Comput. Phys. Commun. 2006; 175:67–71. doi:10.1016/j.cpc.2006.03.007
Scheidemantel TJ, Ambrosch-Draxl C, Thonhauser T, Badding JV, Sofo JO.: Transport coefficients from first-principles calculations. Phys. Rev. B. 2003; 68:125210. doi:10.1103/PhysRevB.68.125210
Ashcroft NW, Mermin ND. Solid State Physics: Holt, Rinehart and Winston; 1976.
Joseph E, Amouyal Y.: Towards a predictive route for selection of doping elements for the thermoelectric compound PbTe from first-principles. J. Appl. Phys. 2015; 117:175102. doi:10.1063/1.4919425
Joseph E, Amouyal Y.: Enhancing thermoelectric performance of PbTe-based compounds by substituting elements: a first principles study. J. Electron. Mater. 2015; 44:1460–1468. doi:10.1007/s11664-014-3416-7
Poudeu PFP, Kanatzidis MG.: Design in solid state chemistry based on phase homologies. Sb4Te3 and Sb8Te9 as new members of the series (Sb2Te3)m·(Sb2)n. Chem. Commun. 2005:2672–2674. doi:10.1039/B500695C
Kifune K, Fujita T, Kubota Y, Yamada N, Matsunaga T.: Crystallization of the chalcogenide compound Sb8Te3. Acta Crystallogr. Sect. B. 2011; 67:381–385. doi:10.1107/S0108768111033738
Amram D, Amouyal Y, Rabkin E.: Encapsulation by segregation – a multifaceted approach to gold segregation in iron particles on sapphire. Acta Mater. 2016; 102:342–351. doi:10.1016/j.actamat.2015.08.081
Ahmad S, Mahanti SD, Hoang K, Kanatzidis MG.: Ab initio studies of the electronic structure of defects in PbTe. Phys. Rev. B. 2006; 74:155205. doi:10.1103/PhysRevB.74.155205
Graff A, Amouyal Y.: Effects of lattice defects and niobium doping on thermoelectric properties of calcium manganate compounds for energy harvesting applications. J. Electron. Mater. 2016; 45:1508–1516. doi:10.1007/s11664-015-4089-6
de Boor J, Stiewe C, Ziolkowski P, Dasgupta T, Karpinski G, Lenz E, Edler F, Mueller E.: High-temperature measurement of seebeck coefficient and electrical conductivity. J. Electron. Mater. 2013; 42:1711–1718. doi:10.1007/s11664-012-2404-z
Edler F, Lenz E.: Metrology for energy harvesting. AIP Conference Proceedings. 2012; 1449:369–372. doi:10.1063/1.4731573
Cowan RD.: Pulse method of measuring thermal diffusivity at high temperatures. J. Appl. Phys. 1963; 34:926–927. doi:10.1063/1.1729564
Rowe DM.: Thermoelectrics Handbook: Macroto Nano. Boca Ravton: Taylor & Francis Group; 2006.
Klemens PG.: The scattering of low-frequency lattice waves by static imperfections. Proc. Phys. Soc. Section A. 1955; 68:1113.
Klemens PG.: Thermal resistance due to point defects at high temperatures. Phys. Rev. 1960; 119:507–509. doi:10.1103/PhysRev.119.507
Abeles B.: Lattice thermal conductivity of disordered semiconductor alloys at high temperatures. Phys. Rev. 1963; 131:1906–1911. doi:10.1103/PhysRev.131.1906
Abeles B, Beers DS, Cody GD, Dismukes JP.: Thermal conductivity of Ge-Si alloys at high temperatures. Phys. Rev. 1962; 125:44–46. doi:10.1103/PhysRev.125.44
Hurd AJ, Kelly RL, Eggert RG, Lee M-H.: Energy-critical elements for sustainable development. MRS Bull. 2012; 37:405–410. doi:10.1557/mrs.2012.54
Callaway J.: Model for lattice thermal conductivity at low temperatures. Phys. Rev. 1959; 113:1046. doi:10.1103/PhysRev.113.1046
Callaway J, von Baeyer HC.: Effect of point imperfections on lattice thermal conductivity. Phys. Rev. 1960; 120:1149. doi:10.1103/PhysRev.120.1149
He J, Zhao L-D, Zheng J-C, Doak J, Wu H, Wang H-Q, Lee Y, Wolverton C, Kanatzidis M, Dravid V.: Role of sodium doping in lead chalcogenide thermoelectrics. J. Am. Chem. Soc. 2013; 135:4624–4627. doi:10.1021/ja312562d
He JQ, Girard SN, Zheng JC, Zhao LD, Kanatzidis MG, Dravid VP.: Strong phonon scattering by layer structured PbSnS2 in PbTe based thermoelectric materials. Adv. Mater. 2012; 24:4440–4444. doi:10.1002/adma.201201565
Kim W, Zide J, Gossard A, Klenov D, Stemmer S, Shakouri A, Majumdar A.: Thermal conductivity reduction and thermoelectric figure of merit increase by embedding nanoparticles in crystalline semiconductors. Phys. Rev. Lett. 2006; 96:045901. doi:10.1103/PhysRevLett.96.045901
Wu LJ, Zheng JC, Zhou J, Li Q, Yang JH, Zhu YM.: Nanostructures and defects in thermoelectric AgPb18SbTe20 single crystal. J. Appl. Phys. 2009; 105: 094317. doi:10.1063/1.3124364
Lo S-H, He J, Biswas K, Kanatzidis MG, Dravid VP.: Phonon scattering and thermal conductivity in p-type nanostructured PbTe-BaTe bulk thermoelectric materials. Adv. Funct. Mater. 2012; 22:5175–5184. doi:10.1002/adfm.201201221
Graff A, Amouyal Y.: Reduced thermal conductivity in niobium-doped calcium-manganate compounds for thermoelectric applications. Appl. Phys. Lett. 2014; 105:181906. doi:10.1063/1.4901269
Goldsmid HJ.: Introduction to Thermoelectricity. Heidelberg Dordrecht London New York: Springer-Verlag; 2009.
Tritt TM. Thermal Conductivity: Theory, Properties, and Applications. Clemson University, Clemson: Kluwer Academic/Plenum Publishers; 2004.
Tritt TM.: Thermoelectric phenomena, materials, and applications. Annu. Rev. Mater. Res. 2011; 41:433–448. doi:10.1146/annurev-matsci-062910-100453
Morelli DT, Heremans JP, Slack GA.: Estimation of the isotope effect on the lattice thermal conductivity of group IV and group III-V semiconductors. Phys. Rev. B. 2002; 66:195304. doi:10.1103/PhysRevB.66.195304
Jovovic V, Heremans JP.: Measurements of the energy band gap and valence band structure of AgSbTe2. Phys. Rev. B. 2008; 77:245204. doi:10.1103/PhysRevB.77.245204
Du BL, Li H, Xu JJ, Tang XF, Uher C.: Enhanced thermoelectric performance and novel nanopores in AgSbTe2 prepared by melt spinning. J. Solid State Chem. 2011; 184:109–114. doi:10.1016/j.jssc.2010.10.036
Medlin DL, Sugar JD.: Interfacial defect structure at Sb2Te3 precipitates in the thermoelectric compound AgSbTe2. Scripta Materialia. 2010; 62:379–382. doi:10.1016/j.scriptamat.2009.11.028
Zhang SN, Zhu TJ, Yang SH, Yu C, Zhao XB.: Phase compositions, nanoscale microstructures and thermoelectric properties in Ag2-ySbyTe1+y alloys with precipitated Sb2Te3 plates. Acta Mater. 2010; 58:4160–4169. doi:10.1016/j.actamat.2010.04.007
Ayral-Marin RM, Brun G, Maurin M, Tedenac JC.: Contribution to the study of AgSbTe2. Euro. J. Solid State Chem. 1990; 27:747–757.
Wu H-J, Chen S-W.: Phase equilibria of Ag–Sb–Te thermoelectric materials. Acta Mater. 2011; 59:6463–6472. doi:10.1016/j.actamat.2011.07.010
Sugar JD, Medlin DL.: Solid-state precipitation of stable and metastable layered compounds in thermoelectric AgSbTe2. J. Mater. Sci. 2011; 46:1668–1679. doi:10.1007/s10853-010-4984-4
Kifune K, Fujita T, Tachizawa T, Kubota Y, Yamada N, Matsunaga T.: Crystal structures of X-phase in the Sb–Te binary alloy system. Cryst. Res. Technol. 2013; 48:1011–1021. doi:10.1002/crat.201300252
Kifune K, Kubota Y, Matsunaga T, Yamada N.: Extremely long period-stacking structure in the Sb-Te binary system. Acta Crystallographica. Section B. 2005; 61:492–497. doi:10.1107/S0108768105017714
Shelimova LE, Karpinskii OG, Kretova MA, Kosyakov VI, Shestakov VA, Zemskov VS, Kuznetsov FA.: Homologous series of layered tetradymite-like compounds in the Sb-Te and GeTe-Sb2Te3 systems. Inorg. Mater. 2000; 36:768–775. doi:10.1007/bf02758595
Sutton AP, Balluffi RW. Interfaces in Crystalline Materials, Oxford: Clarendon Press; 1995.
Porter DA, Easterling KE. Phase Transformations in Metals and Alloys. 2ndEd. London: Chapman & Hall; 1992.
Stowe K.: Crystal structure and electronic band structure of LaTe2. J. Solid State Chem. 2000; 149:155–166. doi:10.1006/jssc.1999.8514
Chen Y, He B, Zhu TJ, Zhao XB.: Thermoelectric properties of non-stoichiometric AgSbTe2 based alloys with a small amount of GeTe addition. J. Phys. D: Appl. Phys. 2012; 45:115302. doi:10.1088/0022-3727/45/11/115302
Chen Y, Nielsen MD, Gao YB, Zhu TJ, Zhao XB, Heremans JP.: SnTe-AgSbTe2 thermoelectric alloys. Adv. Energy Mater. 2012; 2:58–62. doi:10.1002/aenm.201100460
Su T, Jia X, Ma H, Yu F, Tian Y, Zuo G, Zheng Y, Jiang Y, Dong D, Deng L, Qin B, Zheng S.: Enhanced thermoelectric performance of AgSbTe2 synthesized by high pressure and high temperature. J. Appl. Phys. 2009; 105: 3106102. doi:10.1063/1.3106102